arXiv:1605.06869v1 [cond-mat.mtrl-sci] 23 May 2016

Soft X-ray Absorption Spectroscopy Study of Multiferroic Bi-substituted Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3

Hyun Woo Kim, D. H. Kim, Eunsook Lee, and Seungho Seong Department of Physics, The Catholic University of Korea, Bucheon 420-743, Korea

Deok Hyeon Kim and B. W. Lee Department of Physics, Hankuk University of Foreign Studies, Yongin 449-791, Korea

Y. Ko and J.-Y. Kim Pohang Accelerator Laboratory, POSTECH, Pohang 790-784, Korea

J.-S. Kang^∗ Department of Physics, The Catholic University of Korea, Bucheon-si 420-743, Korea (Received)

Abstract

The electronic structures of multiferroic oxides of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12) have been investigated by employing photoemission spectroscopy and soft x-ray absorption spectroscopy (XAS). The measured Fe and Ti 2p XAS spectra show that Ti ions are in the Ti^{4+} states for all x and that Fe ions are Fe^{2+}-Fe^{3+} mixed-valent for x > 0. The valence states of Fe ions are found to be nearly trivalent for x=0, and decreases with increasing x from being nearly trivalent (v(Fe)∼ 3) for x=0 to v(Fe)∼ 2.6 for x=0.12. The valence states of both Ti and Ba ions do not change for all x ≤ 0.12. Based on the obtained valence states of Fe ions, the electronic and magnetic properties of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are explored.

PACS numbers: 78.70.Dm, 75.47.Lx, 79.60.-i Keywords: Multiferroic, XAS, PES, Electronic structure

∗Electronic address: kangjs@catholic.ac.kr; Fax: +82-2-2164-4764

I. INTRODUCTION

Multiferroic materials exhibit the co-existence of multiple ordering, such as ferroelectricity, ferromagnetism, and ferroelasticity.[1] Multiferroic properties observed in manganese (Mn)-based oxides[2] and iron (Fe)-based oxides[3] have stimulated much research on multiferroic transition-metal oxides not only due to the potential technical application but also due to the scientific interest. As an attempt to achieve both ferroelectricity and ferromagnetism, Fe-doped BaTi_{1−x}Fe_xO_3 has been investigated by substituting ferromagnetic Fe ions in hexagonal ferroelectric BaTiO_3.[4–8] Room-temperature ferromagnetism has been observed in BaTi_{1−x}Fe_xO_3 (x < 0.1),[4, 5] and both tetragonal and hexagonal phases exist in BaTi_{1−x}Fe_xO_3 ceramics. The saturation magnetization and the magnetic coercivity were found to depend on the doping level as well as the fraction of the hexagonal phase in the ceramics.[6]. In BaTi_{1−x}Fe_xO_3 system, oxygen vacancy defects and the valence states of the substituted Fe ions are expected to be important in determining the magnetic and ferroelectric properties of the system.[7] However, the reproducibility of multiferroicity and the effect of the oxygen vacancy in BaTi_{1−x}Fe_xO_3 need be investigated more systematically.

Despite extensive studies on multiferroic transition-metal (TM) oxides, the origin of the multiferroicity has not been well understood yet. Based on the XRD (X-ray diffraction) analysis of BaTi_{1−x}Fe_xO_3,[8] the coexistence of Fe^{3+} and Fe^{4+} ions was suggested, implying the availablity of the exchange interactions among Fe^{3+}-Fe^{4+}, Fe^{3+}-Fe^{3+}, and Fe^{4+}- Fe^{4+}. Further, the Fe K-edge XANES (X-ray absorption near-edge structures) study for BaTi_{1−x}Fe_xO_3[9] have shown that both Fe^{3+} and Fe^{4+} ions exist in BaTi_{1−x}Fe_xO_3, with the maximum valence states at x ∼ 0.12. But XRD is not an element-specific experimental method that can determine the valence states of the constituent ions directly. On the other hand, Fe K-edge XANES arises mainly from the Fe 1s → 4p absorption, and so Fe K-edge XANES does not directly represent the Fe 3d configuration in the ground state of Fe ions. Recently, the effect of the simultaneous substitutions of trivalent Bi^{3+} ions for divalent Ba^{2+} ions and trivalent Fe^{3+} (or tetravalent Fe^{4+}) ions for tetravalent Ti^{4+} ions in Ba_{1−x}Bi_xTi_{1−y}Fe_yO_3 has been investigated.[10] Similarly as in BaTi_{1−x}Fe_xO_3, the valence states of Fe ions are expected to play a very important role in Ba_{1−x}Bi_xTi_{1−y}Fe_yO_3. Hence, in order to understand the origin of multiferroicity, it is crucial to determine the valence states of Fe ions directly by using element-specific experimental methods. In this aspect, soft X-ray absorption spectroscopy (XAS) is a powerful experimental tool for studying the valence states of TM ions in solids.[11, 12]

In this work, we have investigated the electronic structures of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12) by employing photoemission spectroscopy (PES) and XAS. PES provides a direct observation of the occupied part of the electronic structures.[13] TM L-edge (2p) XAS involves the 2p → 3d absorption, and so it is a very powerful experimental tool for studying the element-specific valence and spin states of TM ions in solids.[11, 12]

II. EXPERIMENTS DETAILS

Polycrystalline Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12) samples were synthesized by using solid-state reaction methods.[14] PES measurements were performed at the 8A1 beam line, and XAS measurements were performed at both the 8A1 and 2A beam lines of the Pohang Light Source (PLS). The base pressure of the XAS/PES chamber was better than 3 × 10^{−10} Torr. XAS and PES spectra were obtained at room temperature. XAS data were obtained by employing the total electron yield mode with the photon energy resolution of ∼ 100 meV at hν ≈ 600 eV. The overall instrumental resolution of the PES spectra was about ∼ 0.4 eV at hν ∼ 600 eV. All the XAS spectra were normalized to the incident photon flux.

III. RESULTS AND DISCUSSION

Figure 1 shows the survey PES spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 for x=0.1 and 0.12, which are shown in the binding energy (BE) scale. These PES spectra are obtained with hν ≈ 630 eV. Here we have chosen to show the samples with high Bi concentrations because they can reveal both Ba- and Bi-related peaks. All the characteristic core-level peaks of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are observed in the measured survey PES spectra, such as O 1s (∼ 530 eV), Ti 2p (∼ 460 eV), Bi 4f (∼ 160 eV), and Ba 4d (∼ 90 eV) core levels. The large peak around ∼ 290 eV is the C 1s core-level peak, which is often observed in polycrystalline samples. This carbon peak is likely to be due to the impurity carbons present in the grain boundaries of polycrystalline samples, which are not involved in bonding of the solids and do not affect the physical properties the samples. This figure shows that the Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 samples employed in this work are of good quality.

FIG. 1: (Color online) PES survey spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (x=0.1, 0.12), obtained with hν ≈ 630 eV.

Figure 2(a) shows the measured Ti 2p (L-edge) XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (x=0, 0.04, 0.06, 0.1, 0.12) in comparison to that of tetravalent (Ti^{4+}) reference oxide of TiO_2 (our data and [Ref. [15]]. The first two peaks in the low-hν region and the other two peaks in the high-hν region correspond to the Ti L_3 and L_2 peaks, respectively. Here L_3 and L_2 represent the spin-orbit-split 2p_{3/2} (L_3) and 2p_{1/2} (L_2) peaks, which arise from the spin-orbit coupling of the Ti 2p core hole. The Ti 2p XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are found to be nearly identical to one another for all x, indicating that the valence states of Ti ions do not change with x. Further, they are very similar to that of TiO_2, providing evidence that the valence states of Ti ions in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are tetravalent (Ti^{4+}), having the 3d^0 ground-state configuration.

Figure 2(b) shows the measured Ba 3d (M-edge) XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (x=0, 0.04, 0.06, 0.1, 0.12). Here M_5 and M_4 represent the spin-orbit-split 3d_{5/2} and 3d_{3/2} peaks. This comparison shows that the Ba 3d XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are nearly identical to one another for all x. This finding indicates that the valence states of Ba ions do not change with the substitution of Bi ions (x). Since the stable valence states of Ba ions are divalent, the findings of Fig. 2(b) imply that Ba ions are divalent (Ba^{2+}) in

FIG. 2: (Color online) (a) Comparison of the Ti 2p XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 to that of TiO_2 (0 ≤ x ≤ 0.12). (b) Comparison of the Ba 3d XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12).

Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 for x ≤ 0.12.

We now discuss on the valence states of Fe ions in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3. Figure 3(a) shows the measured Fe 2p (L-edge) XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12). As a guide of the valence states of Fe ions, they are compared to those of reference Fe oxides, such as divalent (Fe^{2+}) FeO (Ref. [16, 17]), trivalent (Fe^{3+}) α-Fe_2O_3 (Ref. [16–18]), and and mixed-valent (Fe^{2+}-Fe^{3+}) Fe_3O_4 (Ref. [17]). Similarly as in Ti 2p XAS spectra, L_3 and L_2 peaks represent the spin-orbit-split L_3 (2p_{3/2}) and L_2 (2p_{1/2}) peaks. According to the comparison in Fig. 3(a), the line shapes of the Fe 2p XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are similar to that of α-Fe_2O_3 (Fe^{3+}) but quite different from that of FeO (Fe^{2+}). This observation indicates that Fe ions in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are close to being trivalent (Fe^{3+}), On the other hand, the intensities of the low-hν peak (peak ”A”) with respect to that of the high-hν peak (peak ”B”) in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 are slightly different from that of α- Fe_2O_3. Further, I(A)/I(B (=the relative intensity of peak ”A” to that of peak ”B”) changes

FIG. 3: (Color online) (a) The Fe 2p XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12) in comparison with those of reference Fe oxides of trivalent (Fe^{3+}) α-Fe_2O_3, divalent (Fe^{2+}) FeO, and mixed-valent (Fe^{2+}-Fe^{3+}) Fe_3O_4. (b) Plot of the intensity ratio of Fe L_3 XAS spectra of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 and reference Fe oxides.

slightly for different x values, which is shown better in the relative intensity ratio of I(A)/I(B) in Fig. 3(b). In order to interpret the meaning of I(A)/I(B) values in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3, we examine the lineshapes and I(A)/I(B) of reference Fe oxides. Note that, in divalent (Fe^{2+}) FeO, the peak ”A” is dominant and the peak ”B” appears as a high-hν shoulder. I(A)/I(B) increases from trivalent (Fe^{3+}) α-Fe_2O_3 (0.52) to mixed-valent (Fe^{2+}-Fe^{3+}) Fe_3O_4 (0.63) and divalent (Fe^{2+}) FeO (> 1). This trend is shown more clearly in Fig. 3(b).

Figure 3(b) shows that I(A)/I(B) in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 increases slightly with increasing x. I(A)/I(B) for x=0 is lower than that of α-Fe_2O_3, but I(A)/I(B) for x=0.12 is similar to that of Fe_3O_4. Such a trend in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 and the relative magnitudes with the reference Fe oxides indicate that, in x=0 (BaTi_{0.9}Fe_{0.1}O_3), Fe ions are nearly trivalent (Fe^{3+}), and that, with the substitution of Bi ions for Ba ions (x > 0), the Fe^{2+} component appears, resulting in Fe^{2+}-Fe^{3+} mixed-valent states. For x=0.12 (Ba_{0.88}Bi_{0.12}Ti_{0.9}Fe_{0.1}O_3), the valence states of Fe ions become similar to that of Fe_3O_4 (v(Fe)∼ 2.67). This finding is consistent with the expected trend since Bi ions are generally trivalent (Bi^{3+}) whereas Ba ions are divalent (Ba^{2+}), as confirmed by the measured Ba 3d XAS spectra (see Fig. 2(b)). Considering the charge neutrality conditions in insulating oxides, the substitution of trivalent Bi^{3+} ions for divalent Ba^{2+} ions would cause the decreasing valence states of Fe ions.

Our Fe 2p, Ti 2p, and Ba 3d XAS study on Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 shows that Ti ions are tetravalent (Ti^{4+}) and Ba ions are divalent (Ba^{2+}) for all x in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (x ≤ 0.12). In contrast, with increasing x, the valence states of Fe ions decrease from being nearly trivalent (v(Fe)∼ 3) for x=0 (no Bi ions) to being mixed-valent for x > 0 (Fe^{2+}-Fe^{3+} mixed-valent) and to become v(Fe)∼ 2.6 for x=0.12. This finding refutes the suggestion of the Fe^{3+}-Fe^{4+} mixed-valence states in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3. Hence the idea of the exchange interactions among Fe^{3+}-Fe^{4+}, Fe^{3+}-Fe^{3+}, and Fe^{4+}-Fe^{4+}, need be examined more carefully. This work suggests that the valence states of Fe ions play an important role in determining the electronic and magnetic properties of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3.

IV. CONCLUSIONS

The electronic structures of of multiferroic oxides of Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 (0 ≤ x ≤ 0.12). have been investigated by employing synchrotron-radiation excited PES and XAS. Via Fe and Ti 2p XAS measurements, the valence states of Fe and Ti ions have been determined experimentally. The valence states of Fe ions are found to be Fe^{2+}-Fe^{3+} mixed-valent for x > 0 but nearly trivalent for x=0. The valence states of Fe ions are found to decreases from being nearly trivalent for x=0 (v(Fe)∼ 3) to v(Fe)∼ 2.6 for x=0.12. The valence states of Ti ions do not change with x for x ≤ 0.12, and stay being tetravalent (Ti^{4+}). The valence states of Ba ions are close to being divalent (Ba^{2+}) and remain unchanged for x ≤ 0.12. The decreasing trend of valence states of Fe ions in Ba_{1−x}Bi_xTi_{0.9}Fe_{0.1}O_3 with x will play an important role in the electronic and magnetic properties of this system.

Acknowledgments

This work was supported by the NRF under Contract No. 2014R1A1A2056546, and in part by the Research Fund, 2015 of the Catholic University of Korea. Experiments at PLS were supported by MSIP and PAL.

[1] Y. Tokura and S. Seki, Advanced Materials 22, 1554 (2010).

[2] Y. Kimura, T. Goto, H. Shintani, K Ishizaka, T. Arima and Y. Tokura, Nature 426, 55 (2003). [3] N. Ikeda, H. Ohsumi, K. Ohwada, K. Ishii, T. Inami, K. Kakurai, Y. Murakami, K. Yoshii, S.

Mori, Y. Horibe and H. Kito, Nature (London) 436, 1136 (2005).

[4] A. Rajamani, G. F. Dionne, D. Bono, and C. A. Ross, J. Appl. Phys. 98, 063907 (2005). [5] S. Ray, P. Mahadevan, S. Mandal, S. R. Krishnakumar, C. S. Kuroda, T. Sasaki, T. Taniyama, and M. Itoh, Phys. Rev. B 77, 104416 (2008).

[6] S.-Y. Qiu, W. Li, Y. Liu, G.-H. Liu, Y.-Q. Wu, and N. Chen, Trans. Nonferrous Met. Soc.

China 20, 1911 (2010).

[7] T. Chakraborty, S. Ray, and M. Itoh, Phys. Rev. B 83, 144407 (2011). [8] N. V. Dang, T. D. Thanh, L. V. Hong, V. D. Lam and The-Long Phan, J. Appl. Phys. 110, 043914 (2011).

[9] H. M. Nguyen, N. V. Dang, P.-Y. Chuang, T. D. Thanh, C.-W. Hu, T.-Y. Chen, V. D. Lam C.-H. Lee, and L. V. Hong, Appl. Phys. Lett. 99, 202501 (2011).

[10] D. H. Kim and B. W. Lee, unpublished data (2015).

[11] F. M. F. de Groot, J. C. Fuggle, B. T. Thole, and G. A. Sawatzky, Phys. Rev. B 42, 5459 (1990).

[12] G. van der Laan and I. W. Kirkman, J. Phys.: Condens. Matter 4, 4189 (1992). [13] S. Hüfner, Photoelectron Spectroscopy, Vol. 82 in Solid-State Sciences (Springer-Verlag, Berlin, 1995).

[14] D. H. Kim, M. Y. Lee, Y. M. Kwon, B. W. Lee, Proceedings of International Symposium on Magnetism and Magnetic Materials 2013, MO02, Dec. 5-7, 2013, Phoenix Park, Korea.

[15] L. Soriano, M. Abbate, J. Vogel, J.C. Fuggle, A. Fernandez, A.R. Gonzalez-Elipe, M Sacchi and J.M. Sanz, Surface Sience 290, 427 (1993).

[16] T. J. Regan, H. Ohldag, C. Stamm, F. Nolting, J. Lüning, J. Stöhr, and R. L. White, Phys.

Rev. B 64, 214422 (2001).

[17] K. Küpper, I. Balasz, H. Hesse, A. Winiarski, K. C. Prince, M. Matteucci, D. Wett, R.

Szargan, E. Burzo and M. Neumann, Phys. Stat. Sol. (a) 201, 3252 (2004).

[18] J.-Y. Kim, T. Y. Koo, and J.-H. Park, Phys. Rev. Lett. 96, 047205(2006).